LMucko/crystallography-open-database huggingface dataset:
From isomorphous to “anisomorphous” ionic co-crystals of barbituric acid upon dehydration and return
Maini, L.; Braga, D.; Grepioni, F.; Lampronti, G. I.; Gaglioti, K.; Gobetto, R.; Chierotti, M. R.; CrystEngComm 18 (2016) 4651–; doi:10.1039/C6CE00566G

data_7225093
_publ_section_title
;
 From isomorphous to &#x201C;anisomorphous&#x201D; ionic co-crystals of
 barbituric acid upon dehydration and return
;
_journal_issue                   24
_journal_name_full               CrystEngComm
_journal_page_first              4651
_journal_paper_doi               10.1039/C6CE00566G
_journal_volume                  18
_journal_year                    2016
_chemical_formula_moiety         'C4 H4 N2 O3 K1 Br1'
_chemical_formula_sum            'C4 H4 Br K N2 O3'
_chemical_formula_weight         247.09
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_audit_update_record
;
2016-03-09 deposited with the CCDC.
2016-05-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 97.8638(9)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.3233(5)
_cell_length_b                   7.3226(2)
_cell_length_c                   8.0133(3)
_cell_measurement_temperature    298
_cell_volume                     774.44(5)
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  'Panalytical XPert PRO'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54060
_exptl_crystal_colour            'white powder'
_exptl_crystal_density_diffrn    2.119
_exptl_crystal_description       powder
_pd_char_colour                  white
_pd_proc_ls_prof_R_factor        0.0215
_pd_proc_ls_prof_wR_expected     0.0139
_pd_proc_ls_prof_wR_factor       0.0290
_refine_ls_goodness_of_fit_all   2.09046
_refine_ls_number_parameters     0.000000
_refine_ls_R_I_factor            0.0115
_refine_ls_shift/su_max          0.0173412266
_cod_data_source_file            c6ce00566g2.cif
_cod_data_source_block           BA_NaBr_anhydrous_OKOK_1
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7225093--7225095.cif.
;
_cod_original_sg_symbol_H-M      P121/n1
_cod_database_code               7225093
From isomorphous to “anisomorphous” ionic co-crystals of barbituric acid upon dehydration and return
Maini, L.; Braga, D.; Grepioni, F.; Lampronti, G. I.; Gaglioti, K.; Gobetto, R.; Chierotti, M. R.; CrystEngComm 18 (2016) 4651–; doi:10.1039/C6CE00566G

data_7225094
_publ_section_title
;
 From isomorphous to &#x201C;anisomorphous&#x201D; ionic co-crystals of
 barbituric acid upon dehydration and return
;
_journal_issue                   24
_journal_name_full               CrystEngComm
_journal_page_first              4651
_journal_paper_doi               10.1039/C6CE00566G
_journal_volume                  18
_journal_year                    2016
_chemical_formula_moiety         'C4 H4 N2 O3 Na1 Br1'
_chemical_formula_sum            'C4 H4 Br N2 Na O3'
_chemical_formula_weight         230.98
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_audit_update_record
;
2016-03-09 deposited with the CCDC.
2016-05-04 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 102.141(2)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   14.1395(6)
_cell_length_b                   7.3740(3)
_cell_length_c                   13.9831(6)
_cell_measurement_temperature    298
_cell_volume                     1425.33(10)
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  'Panalytical XPert PRO'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.54060
_exptl_crystal_colour            'white powder'
_exptl_crystal_density_diffrn    2.153
_exptl_crystal_description       powder
_pd_char_colour                  white
_pd_proc_ls_prof_R_factor        0.0756
_pd_proc_ls_prof_wR_expected     0.0118
_pd_proc_ls_prof_wR_factor       0.1048
_refine_ls_goodness_of_fit_all   8.84972
_refine_ls_number_parameters     0.000000
_refine_ls_R_I_factor            0.0649
_refine_ls_shift/su_max          2.29884712e-017
_cod_data_source_file            c6ce00566g2.cif
_cod_data_source_block           BA_NaBr_anhydrous_OKOK
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_diffrn_radiation_probe' value 'X-ray' changed to 'x-ray' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7225093--7225095.cif.
;
_cod_original_sg_symbol_H-M      C2/c
_cod_original_formula_sum        'C4 H4 N2 O3 Na1 Br1'
_cod_database_code               7225094
Usnic Acid Derivatives with Cytotoxic and Antifungal Activities from the Lichen Usnea longissima.
Yu, Xuelong; Guo, Qiang; Su, Guozhu; Yang, Ailin; Hu, Zhongdong; Qu, Changhai; Wan, Zhe; Li, Ruoyu; Tu, Pengfei; Chai, Xingyun; Journal of natural products 79 (2016) 1373–1380; doi:10.1021/acs.jnatprod.6b00109

data_1543335
_publ_section_title
;
 Usnic Acid Derivatives with Cytotoxic and Antifungal Activities from the
 Lichen Usnea longissima.
;
_journal_issue                   5
_journal_name_full               'Journal of natural products'
_journal_page_first              1373
_journal_page_last               1380
_journal_paper_doi               10.1021/acs.jnatprod.6b00109
_journal_volume                  79
_journal_year                    2016
_chemical_formula_sum            'C18 H17 N O6'
_chemical_formula_weight         343.330
_space_group_IT_number           1
_symmetry_Int_Tables_number      1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_audit_creation_date             2015-05-21
_audit_creation_method
'Olex2 1.1 (compiled 2011.02.15 svn.r1672, GUI svn.r3494)''
_audit_update_record             2015-05-21
_cell_angle_alpha                90.000
_cell_angle_beta                 134.45(3)
_cell_angle_gamma                90.000
_cell_formula_units_Z            1
_cell_length_a                   17.138(2)
_cell_length_b                   9.7525(5)
_cell_length_c                   13.831(2)
_cell_volume                     1650.2(9)
_refine_ls_R_factor_all          0.034
_cod_data_source_file            np6b00109_si_002.cif
_cod_data_source_block           exp_2842
_cod_depositor_comments
;
Adding full bibliography for 1543335--1543336.cif.

2019-03-17
Fixing wrong Z value.                 miguel
;
_cod_original_cell_volume        1650.2(4)
_cod_original_sg_symbol_Hall     P_1
_cod_original_formula_units_Z    4
_cod_database_code               1543335
Usnic Acid Derivatives with Cytotoxic and Antifungal Activities from the Lichen Usnea longissima.
Yu, Xuelong; Guo, Qiang; Su, Guozhu; Yang, Ailin; Hu, Zhongdong; Qu, Changhai; Wan, Zhe; Li, Ruoyu; Tu, Pengfei; Chai, Xingyun; Journal of natural products 79 (2016) 1373–1380; doi:10.1021/acs.jnatprod.6b00109

data_1543336
_publ_section_title
;
 Usnic Acid Derivatives with Cytotoxic and Antifungal Activities from the
 Lichen Usnea longissima.
;
_journal_issue                   5
_journal_name_full               'Journal of natural products'
_journal_page_first              1373
_journal_page_last               1380
_journal_paper_doi               10.1021/acs.jnatprod.6b00109
_journal_volume                  79
_journal_year                    2016
_chemical_formula_sum            'C20 H23 N O7'
_chemical_formula_weight         389.390
_space_group_IT_number           1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_audit_creation_date             2015-05-21
_audit_creation_method
'Olex2 1.1 (compiled 2011.02.15 svn.r1672, GUI svn.r3494)''
_audit_update_record             2015-05-21
_cell_angle_alpha                90.000
_cell_angle_beta                 93.840(1)
_cell_angle_gamma                90.000
_cell_formula_units_Z            4
_cell_length_a                   11.6293(2)
_cell_length_b                   9.9961(2)
_cell_length_c                   16.9428(2)
_cell_volume                     1965.14(6)
_refine_ls_R_factor_all          0.034
_cod_data_source_file            np6b00109_si_003.cif
_cod_data_source_block           exp_2874
_cod_depositor_comments
'Adding full bibliography for 1543335--1543336.cif.'
_cod_original_cell_volume        1965.2(1)
_cod_database_code               1543336
Structure de SrTeO~4~ sur monocristal. Organisation de structures comportant des empilements de chaînes (TeO~4~)~n~. Dimorphisme de Na~2~TeO~4~
Lapasset, J.; Moret, J.; Acta Crystallographica, Section C: Crystal Structure Communications 41 (1985) 1558–1562; doi:10.1107/s0108270185008551

data_2020520
_publ_section_title
;
 Structure de SrTeO~4~ sur monocristal. Organisation de structures comportant
 des empilements de cha\^ines (TeO~4~)~n~. Dimorphisme de Na~2~TeO~4~
;
_journal_issue                   11
_journal_name_full
;
 Acta Crystallographica, Section C: Crystal Structure Communications
;
_journal_page_first              1558
_journal_page_last               1562
_journal_paper_doi               10.1107/s0108270185008551
_journal_volume                  41
_journal_year                    1985
_chemical_formula_structural     'Sr Te O4'
_chemical_formula_sum            'O4 Sr Te'
_chemical_name_systematic        'Strontium tellurate'
_space_group_IT_number           60
_symmetry_Int_Tables_number      60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90.
_cell_angle_beta                 90.
_cell_angle_gamma                90.
_cell_formula_units_Z            4
_cell_length_a                   5.605(3)
_cell_length_b                   13.181(4)
_cell_length_c                   5.003(2)
_cell_measurement_temperature    295.
_cell_volume                     369.6(3)
_cod_data_source_file            SrTeO4_Pbcn_DC287.cif
_cod_data_source_block           chateigner
_cod_original_cell_volume        369.62
_cod_original_formula_sum        'O4 Sr1 Te1'
_cod_database_code               2020520
Nitrogen-rich hypergolic ionic salts based on (2-methyltetrazol-5-yl)diazotates
chen, fuxue; Wang, Qi; Lu, Huijie; Pang, Fu-Qing; Huang, Jinglun; Nie, Fude; RSC Adv.  (2016) –; doi:10.1039/C6RA11494F

data_7225499
_publ_section_title
;
 Nitrogen-rich hypergolic ionic salts based on
 (2-methyltetrazol-5-yl)diazotates
;
_journal_name_full               'RSC Adv.'
_journal_paper_doi               10.1039/C6RA11494F
_journal_year                    2016
_chemical_formula_sum            'C3 H10 N10 O'
_chemical_formula_weight         202.210
_space_group_IT_number           2
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_audit_creation_date             15-09-30
_audit_creation_method           'Created with Diamond (www.crystalimpact.com)'
_audit_update_record
;
2015-10-13 deposited with the CCDC.
2016-06-07 downloaded from the CCDC.
;
_cell_angle_alpha                84.83(2)
_cell_angle_beta                 82.81(2)
_cell_angle_gamma                83.49(2)
_cell_formula_units_Z            2
_cell_length_a                   3.805(3)
_cell_length_b                   7.898(6)
_cell_length_c                   15.015(11)
_cell_volume                     443.5(6)
_refine_ls_R_factor_all          0.086
_cod_data_source_file            c6ra11494f2.cif
_cod_data_source_block           bo3424
_cod_original_sg_symbol_Hall     -P_1
_cod_database_code               7225499
Crystal structure of thalium(I) 2-thiobarbiturate
N.N. Golovnev; M.S. Molokeev; Russian Journal of Inorganic Chemistry 61 (2016) 463–467; doi:10.1134/S0036023616040100

data_4031992
_publ_section_title
;
 Crystal structure of thalium(I) 2-thiobarbiturate
;
_journal_issue                   4
_journal_name_full               'Russian Journal of Inorganic Chemistry'
_journal_page_first              463
_journal_page_last               467
_journal_paper_doi               10.1134/S0036023616040100
_journal_volume                  61
_journal_year                    2016
_chemical_formula_moiety         'C4 H3 N2 O2 S Tl'
_chemical_formula_sum            'C4 H3 N2 O2 S Tl'
_chemical_formula_weight         347.5317
_space_group_IT_number           13
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yc'
_symmetry_space_group_name_H-M   'P 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.4520(24)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.24141(73)
_cell_length_b                   3.94441(25)
_cell_length_c                   14.83809(88)
_cell_measurement_temperature    300
_cell_volume                     649.00(7)
_diffrn_ambient_temperature      300
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    50.345
_exptl_crystal_density_diffrn    3.556804
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.0160352
_pd_meas_2theta_range_max        99.9925248
_pd_meas_2theta_range_min        5
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 6 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.900
_pd_proc_ls_prof_wR_expected     4.471
_pd_proc_ls_prof_wR_factor       6.492
_pd_proc_number_of_points        5924
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   1.452
_refine_ls_R_I_factor            1.379
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            TlHTBA.cif
_cod_data_source_block           a
_cod_original_cell_volume        648.999(70)
_cod_original_sg_symbol_Hall
;
-P 2yc
;
_cod_original_sg_symbol_H-M      P2/c
_cod_original_formula_sum
;
C4 H3 N2 O2 S Tl
;
_cod_database_code               4031992
_cod_database_fobs_code          4031992
The crystal structure of K2VO2F3, a nonlinear dioxovanadium(V) group
Ryan, R. R.; Mastin, S. H.; Reisfeld, M. J.; Acta Crystallographica Section B Structural Crystallography and Crystal Chemistry 27 (1971) 1270–1274; doi:10.1107/s0567740871003844

data_2020524
_publ_section_title
;
 The crystal structure of K2VO2F3, a nonlinear dioxovanadium(V) group
;
_journal_issue                   6
_journal_name_full
'Acta Crystallographica Section B Structural Crystallography and Crystal Chemistry'
_journal_page_first              1270
_journal_page_last               1274
_journal_paper_doi               10.1107/s0567740871003844
_journal_volume                  27
_journal_year                    1971
_chemical_formula_sum            'F3 K2 O2 V'
_space_group_IT_number           62
_space_group_name_Hall           '-P 2ac 2n'
_space_group_name_H-M_alt        'P n m a'
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.379(4)
_cell_length_b                   5.640(2)
_cell_length_c                   11.413(7)
_cell_measurement_radiation      'Mo K\a~1~'
_cell_measurement_reflns_used    12
_cell_volume                     475.0(4)
_diffrn_radiation_type           'Mo K\a'
_refine_ls_matrix_type           full
_refine_ls_number_reflns         668
_refine_ls_R_factor_all          0.0258
_refine_ls_shift/su_max          0.001
_refine_ls_wR_factor_all         0.0198
_reflns_threshold_expression     I>2.5u(I)
_cod_data_source_file            Ryan1971.cif
_cod_data_source_block           Ryan1971
_cod_database_code               2020524
Sr3TeO6 and Ba3TeO6: double perovskites with pronounced superstructures
Stöger, Berthold; Weil, Matthias; Zobetz, Erich; Zeitschrift für Kristallographie 225 (2010) 125–138; doi:10.1524/zkri.2010.1234

data_8104519
_publ_section_title
;
 Sr3TeO6 and Ba3TeO6: double perovskites with pronounced superstructures
;
_journal_name_full               'Zeitschrift f\"ur Kristallographie'
_journal_page_first              125
_journal_page_last               138
_journal_paper_doi               10.1524/zkri.2010.1234
_journal_volume                  225
_journal_year                    2010
_chemical_formula_sum            'Ba3 O6 Te'
_chemical_formula_weight         635.62
_space_group_IT_number           88
_symmetry_space_group_name_Hall  '-I 4ad'
_symmetry_space_group_name_H-M   'I 41/a :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            80
_cell_length_a                   19.3878(10)
_cell_length_b                   19.3878(10)
_cell_length_c                   34.909(2)
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      40.52
_cell_measurement_theta_min      2.33
_cell_volume                     13121.8(12)
_diffrn_reflns_number            146437
_exptl_crystal_size_max          0.05
_exptl_crystal_size_min          0.05
_refine_ls_extinction_coef       0.0000038(2)
_refine_ls_extinction_method     SHELXL
_refine_ls_number_parameters     453
_refine_ls_R_factor_gt           0.034
_refine_ls_wR_factor_all         0.06
_reflns_threshold_expression     F^2^>u(F)
_cod_data_source_file            Ba3TeO6.cif
_cod_data_source_block           Ba3TeO6
_cod_original_sg_symbol_Hall     'I 41/a'
_cod_original_sg_symbol_H-M      '-I 4ad'
_cod_database_code               8104519
Sr3TeO6 and Ba3TeO6: double perovskites with pronounced superstructures
Stöger, Berthold; Weil, Matthias; Zobetz, Erich; Zeitschrift für Kristallographie 225 (2010) 125–138; doi:10.1524/zkri.2010.1234

data_8104520
_publ_section_title
;
 Sr3TeO6 and Ba3TeO6: double perovskites with pronounced superstructures
;
_journal_name_full               'Zeitschrift f\"ur Kristallographie'
_journal_page_first              125
_journal_page_last               138
_journal_paper_doi               10.1524/zkri.2010.1234
_journal_volume                  225
_journal_year                    2010
_chemical_formula_sum            'O6 Sr3 Te'
_chemical_formula_weight         486.46
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-F 1'
_space_group_name_H-M_alt        'F -1'
_cell_angle_alpha                90.031(2)
_cell_angle_beta                 90.035(2)
_cell_angle_gamma                90.1370(10)
_cell_formula_units_Z            32
_cell_length_a                   16.5338(2)
_cell_length_b                   16.6308(2)
_cell_length_c                   16.7112(3)
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      45.31
_cell_measurement_theta_min      2.12
_cell_volume                     4595.07(11)
_diffrn_reflns_number            72318
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.1
_refine_ls_extinction_coef       0.000250(5)
_refine_ls_extinction_method     SHELXL
_refine_ls_number_parameters     375
_refine_ls_R_factor_gt           0.035
_refine_ls_wR_factor_all         0.076
_reflns_threshold_expression     F^2^>u(F)
_cod_data_source_file            Sr3TeO6.cif
_cod_data_source_block           Sr3TeO6
_cod_depositor_comments
;
 Updating space group information.

 2018-06-13,
 Antanas Vaitkus
;
_cod_database_code               8104520
Dinuclear Silver(I) and Copper(II) Complexes of Hexadentate Macrocyclic Ligands Containing p-Xylyl Spacers
McKenzie, Christine J.; Nielsen, Lars Preuss; Sotofte, Inger; Acta Chemica Scandinavica 52 (1998) 571–577; doi:10.3891/acta.chem.scand.52-0571

data_1543492
_publ_section_title
;
 Dinuclear Silver(I) and Copper(II) Complexes of Hexadentate Macrocyclic
 Ligands Containing p-Xylyl Spacers
;
_journal_name_full               'Acta Chemica Scandinavica'
_journal_page_first              571
_journal_page_last               577
_journal_paper_doi               10.3891/acta.chem.scand.52-0571
_journal_volume                  52
_journal_year                    1998
_chemical_formula_sum            'C30 H42 Ag2 N6 O6'
_chemical_formula_weight         826.46
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 97.53(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.153(6)
_cell_length_b                   12.263(4)
_cell_length_c                   9.220(2)
_cell_volume                     1586.4(9)
_diffrn_ambient_temperature      120
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_exptl_absorpt_coefficient_mu    1.288
_exptl_crystal_density_diffrn    1.73
_exptl_crystal_F_000             840
_refine_ls_goodness_of_fit_ref   1.10
_refine_ls_number_parameters     292
_refine_ls_number_reflns         3646
_refine_ls_R_factor_gt           0.0367
_refine_ls_wR_factor_ref         0.0699
_cod_data_source_file            Acta-Chem-Scand-1998-52-571-577.cif
_cod_data_source_block           1
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_original_formula_sum        'C30 H42 N6 O6 Ag2'
_cod_database_code               1543492